Mechanics Research Communications 47 (2013) 102–105 Contents lists available at SciVerse ScienceDirect Mechanics Research Communications journal homepage: www.elsevier.com/locate/mechrescom Singularities in auxetic elastic bimaterials M.M. Adam a , J.R. Berger a,∗ , P.A. Martin b a b Department of Mechanical Engineering, Colorado School of Mines, Golden, CO 80401, USA Department of Applied Mathematics and Statistics, Colorado School of Mines, Golden, CO 80401, USA a r t i c l e i n f o Article history: Received 27 September 2012 Received in revised form 2 October 2012 Accepted 4 October 2012 Available online 11 October 2012 Keywords: Auxetic material Bimaterials singularities a b s t r a c t In this paper we study the effects of negative Poisson’s ratios on elastic problems containing singularities. Materials with a negative Poisson’s ratio are termed auxetic. We present a brief review of such materials. The elasticity problem of a bimateral wedge is presented, then two particular cases of this problem are investigated: the free-edge problem and the interface crack problem. We study the effect on the stress singularity due to one portion of the bimaterial becoming auxetic. We find that the auxetic material has a significant effect on the singularity order, even causing the singularity to vanish for certain values of the elastic constants. © 2012 Elsevier Ltd. All rights reserved. 1. Introduction Poisson observed that a material stretched under axial tensile forces not only elongates longitudinally, but it also contracts laterally. Most common materials undergo a transverse contraction when stretched in one direction and a transverse expansion when compressed; the magnitude of this transverse deformation is governed by Poisson’s ratio. Poisson’s ratio has two theoretical limits for a linear elastic, isotropic material: −1 < < 0.5. The upper limit, → 0.5, represents the incompressible limit for the material, and the lower limit, → −1, is required for the strain energy to be a positive definite function (Fung et al., 1965). Lakes (1987) presented a new foam structure which exhibited a negative Poisson’s ratio. This was achieved by converting a conventional foam using heating and compression techniques to create a reentrant structure. This type of material is called auxetic: the material expands laterally upon longitudinal tensile loading and contracts laterally under longitudinal compression. Auxetic materials are not completely new: Love (1944) in his treatise book on elasticity presents an example of “single crystal pyrite” with a Poisson’s ratio of −1/7. However, this material is cubic and Poisson’s ratios do not follow the isotropic limits. For anisotropic solids, no such limits exist as shown by Ting and Chen (2005). Auxetic materials are very rare in nature as discussed by Stavroulakis (2005). Some examples are silicon polymorphs (Kimizuka et al., 2000; Yeganeh-Haeri et al., 1992;Alderson and ∗ Corresponding author. Tel.: +1 303 273 3682. E-mail addresses: madam@mines.edu (M.M. Adam), jberger@mines.edu (J.R. Berger), pamartin@mines.edu (P.A. Martin). 0093-6413/$ – see front matter © 2012 Elsevier Ltd. All rights reserved. http://dx.doi.org/10.1016/j.mechrescom.2012.10.003 Evans, 2002; Keskar and Chelikowsky, 1992), zeolite (Grima et al., 2005), and silicates (Grima et al., 2005). Additionally, auxetic behavior can be created in foams and similar materials by varying the geometric structure (Grima and Evans, 2000, 2006; Smith et al., 2000; Grima et al., 2012). The auxetic behavior in these materials can be explained in terms of their geometry and deformation mechanisms. Auxetic behavior has also been observed to occur locally on the nanoscale in certain materials (Alderson et al., 2005; Franke and Magerle, 2011), and auxetic behavior has been noted in certain plate problems (Bhullar et al., 2010). A review article by Yang et al. (2004) summarizes much of the state of the art as to current understanding of both natural and man-made auxetic materials. The effects of auxetic behavior on material properties have been investigated (see, for example, Lakes and Drugan, 2002) to study if material properties such as hardness, toughness, indentation resistance, and acoustic response can be enhanced. For example, in Lakes (1987) and Grima and Evans (2000) the shear modulus, , is predicted to increase as the Poisson’s ratio approaches the lower theoretical limit ( → −1.0) if Young’s modulus (E) is constant. Indentation resistance has been investigated and enhancements in hardness have been found. Auxetic foams have been found to be up to three times more difficult to indent than conventionally processed polymers (Alderson et al., 2000). Foams with negative Poisson’s ratios were also found to have higher resilience than conventional foams (Lakes, 1987). Finally, auxetic materials are predicted to become very tough according to classical elasticity theory when the Poisson’s ratio approaches the lower limit of −1.0. For example, the fracture toughness of negative Poisson’s ratio open cell copper foams are enhanced by 80%, 130%, and 160% for permanent volumetric compression ratio values of 2.0, 2.5 and 3.0, respectively, compared to a conventional foam with a positive Poisson ratio (Choi and Lakes, 1996). M.M. Adam et al. / Mechanics Research Communications 47 (2013) 102–105 103 in the stress field on the wedge angles and the elastic constants of the materials was also investigated by Hein and Erdogan (1971). Numerical results of several angle geometries for all relevant material constants combinations were produced. Finally, we note that Green’s function methods have also been used successfully on the free-edge problem. The anisotropic problem was considered by Tewary (1991), where the Green’s function was represented by an exact integral. Both the displacement and the stress Green’s function were obtained. A Green’s function method was also employed by Martin (2003) where a reduced equation for calculating the singularity order was found. An anisotropic bimaterial problem was also considered by Berger et al. (1998) where it was noted that the free edge singularity vanishes for certain free-surface angles and elastic constants combinations. 3. Formulation In this section, we review the analytical solution for the bimaterial wedge as introduced in previous papers, see for example Bogy (1968), Ding and Kumosa (1994). To be definite, we consider plane-strain problems; similar results are available for plane-stress problems. Typical solutions use an Airy stress function in polar coordinates, (r, ) (Williams, 1952), written in each portion of the bimaterial, Fig. 1. General elastic bimaterial problem. The motivation for the present paper is to investigate problems in elastic bimaterials when one portion of the bimaterial is auxetic. Typical problems of this nature are the free-edge singularity (which can be useful in investigating delaminatation failures in bimaterials) and the interface crack problem. To generalize the problem, we present results for both the free-edge and interface crack problems over the entire range of permissible Poisson ratios where the effect of a material becoming auxetic on the stress singularity order may be readily seen. j (r, ) We consider the general bimaterial problem shown in Fig. 1. Both Material 1 and Material 2 are taken to be linear, elastic, isotropic, and homogeneous. Material j has Poisson’s ratio j , shear modulus j , and Young’s modulus Ej , j = 1, 2. We will assume the two materials are perfectly bonded at the planar interface so displacements and tractions are continuous across the interface. The local polar coordinate system r, is positioned at the root of the notch, and the notch-face angle is assumed to be symmetric with respect to the interface. We focus on two specific problems: the free-edge problem ( = /2 in Fig. 1) and the interface crack problem ( = ). Of particular interest in both problems is the nature of the increase in stress (if any) as r → 0. The singularity order ı has been studied extensively in isotropic bimaterials. For interface cracks, solutions of the type ∼ rı have been obtained where ı is complex valued. The free-edge problem has been extensively studied by Bogy (1968, 1970) and others, and the stress field solution was of the type rı where ı was realvalued depending on the elastic properties of the two materials. Dundurs (1969) reduced the number of parameters that the stress field depends on from three to two and used these parameters to express the solution in a more compact way. The plane problem of bonded dissimilar wedges of arbitrary angle subjected to general forms of loading was studied by Hein and Erdogan (1971). The solution was obtained by solving two simpler problems where the solution is given by the sum of solutions of the two separated problems. The dependence of singularity order j = 1, 2 (1) where Fj () can be determined from the governing differential equation for , ∇ 4 = 0. The stress components in each portion of the bimaterial are then (j) rr = (ı + 1)r ı ı[Aj sin ı − Bj cos ı] (2) −(ı + 2)[Cj sin(ı + 2) + Dj cos(ı + 2)] , (j) r = (ı + 1)r ı ı[Aj cos ı + Bj sin ı] (3) +(ı + 2)[Cj cos(ı + 2) − Dj sin(ı + 2)] , (j) 2. Singularities in bimaterials = r ı Fj (), = (ı + 1)(ı + 2)r ı Aj sin ı + Bj cos ı (4) +Cj sin(ı + 2) + Dj cos(ı + 2) , where j = 1, 2 indicates if the stress component is in Material 1 or 2. Using similar notation, the displacements in each portion of the bimaterial are (j) ur = r ı+1 Ej ı + j (ı + 2) [Aj sin ı − Bj cos ı] (5) −(ı + 2)(1 + j )[Cj sin(ı + 2) + Dj cos(ı + 2)] , (j) u = r ı+1 {−(j (ı + 2) + (ı + 6))[Aj cos ı + Bj sin ı] Ej (6) +(ı + 2)(1 + j )[Cj cos(ı + 2) + Dj sin(ı + 2)]}. For continuity of displacement and traction at the interface, = 0, (1) (2) u (r, 0) = u (r, 0), (1) (2) r (r, 0) = r (r, 0). ur (r, 0) = ur (r, 0), (r, 0) = (r, 0), (1) (2) (1) (2) (7) (8) Finally, the traction-free surface conditions are (1) (2) (1) (2) (r, ) = (r, −) = r (r, ) = r (r, −) = 0. (9) Substituting the stress and displacement equations in the boundary and continuity conditions, we obtain eight linear equations in the eight unknown values of Aj , Bj , Cj , and Dj which can be written in matrix form as Ax = 0. For a non-trivial solution we then have det A = 0, which yields the singularity order ı. 104 M.M. Adam et al. / Mechanics Research Communications 47 (2013) 102–105 Fig. 2. Singularity order ı for the free-edge problem as a function of 1 (with 2 = 0.30) for 2 ≤ E = E1 /E2 ≤ 1000. Fig. 3. Singularity order ı for the free-edge problem as a function of 1 (with 2 = 0.30) for 1.5 ≤ E ≤ 4.5. 5. The interface crack problem 4. The free-edge problem For this problem, we consider the effects of an auxetic material on the singularity at the intersection between an interface and the free surface of the bimaterial. Following Martin (2003), the singularity order for = /2 can be computed from det A = −44 (ı + 1)2 [(1 − 1 )2 + (1 − 2 )1 ]2 (ı) = 0 2 +(ı + 1) (ı + 1)2 (˛ − ˇ)2 − ˛ 2 (13) where the second term arises from the imaginary part of the singularity order and is usually referred to in the literature as the oscillatory part of the singularity. This can be computed in planestrain as (Gu and Belytschko, 1994) as (11) Im(ı) = = (ˇ2 − 1)S 4 + 1 + 2(ı + 1)2 (˛ − ˇ)ˇ S 2 ∼r −1/2 cos(Im(ı) log r) (10) where (ı) For this problem, we investigate the effect of an auxetic material on the singularity at the tip of an interface crack, that is, when = . The stress field near the tip of the crack varies, for example, as (Atkinson, 1979) , 1 (3 − 41 )2 + 1 . log 2 (3 − 42 )1 + 2 (14) (12) When the two portions of the bimaterial are closely matched elastically, the imaginary part of the singularity order is very small as expected. In Fig. 4 we have plotted Im(ı) for a variety of ratios 1 /2 as a function of 1 . As with the free-edge problem, we have kept 2 = 0.30 for these calculations. We note in the figure that, in In the majority of the literature (see, for example, Hutchinson and Suo, 1992), physically admissible values for the Dundurs constants are restricted to lie within the parallelogram enclosed by ˛ = ±1 and ˛ − 4ˇ = ±1 in the (˛, ˇ) plane. However, this result assumes that Poisson’s ratio is positive. If we permit auxetic materials, the parallelogram is 50% larger; it is enclosed by ˛ = ±1 and ˛ − 83 ˇ = ±1. To examine the influence of one portion of the bimaterial becoming auxetic, we calculate the singularity order, ı, from Eq. (11) as we vary 1 . For this calculation we fix 2 = 0.30 and allow the elastic moduli ratio, E = E1 /E2 , to vary. The first set of results is shown in Fig. 2, where we plot ı as a function of 1 . We take values of 1 across the entire range of permissible values of the Poisson ratio, −1 < 1 < 0.5. Note in the figure that the singularity order, ı, becomes increasingly negative as E is increased for fixed 1 . Also, once Material 1 becomes auxetic (1 < 0), the singularity order is significantly affected by the Poisson ratio. In certain cases the singularity order decreases over 18% due to Material 1 becoming auxetic. Finally, in Fig. 2 we note that for E = 2, the singularity disappears when 1 decreases below −0.4. This is explored in more detail in Fig. 3 for moduli ratios of 1.5 ≤ E ≤ 4.5. In Fig. 3, note that if E ≥ 3, the singularity cannot be eliminated. Fig. 4. Imaginary part of the singularity order ı for the interface crack problem as a function of 1 (with 2 = 0.30) for 1.5 ≤ E1 /E2 ≤ 1000. S = − sin 12 (ı + 1), and ˛, ˇ are Dundurs constants (Dundurs, 1969); for plane-strain problems, ˛= E−1 , E+1 ˇ= (1 − 22 )1 − (1 − 21 )2 , 2(1 − 2 )1 + 2(1 − 1 )2 E= E1 . E2 M.M. Adam et al. / Mechanics Research Communications 47 (2013) 102–105 105 Table 1 Values of 1 where Im(ı) = 0 (2 = 0.3). 1 /2 1 1.5 0.2 2.0 0.1 2.5 0.0 3.0 −0.1 3.5 −0.2 4.0 −0.3 general, a negative Poisson’s ratio causes the oscillatory singularity to decrease when compared to cases where the Poisson’s ratio is positive. Of particular interest are cases where the decrease due to 1 becoming negative can actually drive Im(ı) to zero. In Table 1 we present values for 1 where Im(ı) = 0 for various ratios 1 /2 . Note in the table that if 1 /2 > 2.5, the material must be auxetic in order for the crack-tip singularity to be purely real. 6. Summary In this paper, we have investigated stress singularities in elastic bimaterials where we allow the Poisson’s ratio of one portion of the bimaterial to vary completely over −1 < < 0.5. Our motivation for this study comes from recent discoveries of auxetic materials, and how this might affect stress singularities in such problems. We found that when one portion of the bimaterial becomes auxetic, the effect on either the free-edge or interface crack singularity can be profound, even causing it to vanish given appropriate values of the remaining elastic constants. As more auxetic materials are developed, this fact could lead to strategies helping to suppress delamination or fracture failures in these bimaterials. Acknowledgements The authors acknowledge the support of the Army Research Office, grant number DAAD19-01-1-0590, to the Colorado School of Mines. Helpful discussions with Prof. I. Reimanis of the Department of Metallurgical and Materials Engineering at the Colorado School of Mines are gratefully acknowledged. References Alderson, A., Evans, K.E., 2002. Molecular origin of auxetic behavior in tetrahedral framework silicates. Physical Review Letters 89, 225503–225507. Alderson, K.L., Fitzgerald, A., Evans, K.E., 2000. The strain dependent indentation resilience of auxetic microporous polyethylene. Journal of Materials Science 35, 4039–4047. Alderson, A., Alderson, K.L., Evans, K.E., Grima, J.N., Williams, M.R., Davies, P.J., 2005. Modeling the deformation mechanisms, structure-property relationships and applications of auxetic nanomaterials. Physical Status Solidi B 242, 499–508. Atkinson, C., 1979. Stress singularities and fracture mechanics. Applied Mechanics Reviews 32, 123–135. Berger, J.R., Martin, P.A., Lien, J.P., 1998. Reduction of free-edge stress intensities in anisotropic bi-materials. International Journal of Fracture 91, 165–177. Bhullar, S.K., Wegner, J.L., Mioduchowski, A., 2010. Auxetic behavior of a thermoelastic layered plate. Journal of Engineering and Technology Research 2, 161–167. Bogy, D.B., 1968. Edge-bonded dissimilar orthogonal elastic wedges under normal and shear loading. Journal of Applied Mechanics 35, 460–466. 4.5 −0.4 5.0 −0.5 5.5 −0.6 6.0 −0.7 6.5 −0.8 7.0 −0.9 Bogy, D.B., 1970. On the problem of edge-bonded elastic quarter-planes loaded at the boundary. International Journal of Solids and Structures 6, 1287–1313. Choi, J.B., Lakes, R.S., 1996. Fracture toughness of re-entrant foam materials with a negative Poisson’s ratio: experiment and analysis. International Journal of Fracture 80, 73–83. Ding, S., Kumosa, M., 1994. Singular stress behavior at an adhesive interface corner. Engineering Fracture Mechanics 47, 503–519. Dundurs, J., 1969. Discussion of Bogy (1968). Journal of Applied Mechanics 36, 650–651. Franke, M., Magerle, R., 2011. Locally auxetic behavior of elastometric polypropylene on the 100 nm length scale. ACS Nano 5, 4886–4891. Fung, Y.C., 1965. Foundations of Solid Mechanics. Prentice Hall, Englewood Cliffs, NJ. Grima, J.N., Evans, K.E., 2000. Auxetic behavior from rotating squares. Journal of Materials Science Letters 19, 1563–1565. Grima, J.N., Evans, K.E., 2006. Auxetic behavior from rotating triangles. Journal of Materials Science 41, 3193–3196. Grima, J.N., Gatt, R., Alderson, A., Evans, K.E., 2005. On the origin of auxetic behavior in the silicate ˛-cristobalite. Journal of Materials Chemistry 15, 4003–4005. Grima, J.N., Chetcuti, E., Manicardo, E., Attard, D., Camilleri, M., Gatt, R., 2012. On the auxetic properties of generic rotating rigid triangles. Proceeding of the Royal Society A 468, 810–830. Gu, L., Belytschko, T., 1994. A numerical study of stress singularities in a two-material wedge. International Journal of Solids and Structures 31, 865–889. Hein, V.L., Erdogan, F., 1971. Stress singularities in a two-material wedge. International Journal of Fracture Mechanics 7, 317–330. Hutchinson, J.W., Suo, Z., 1992. Mixed mode cracking in layered materials. Advances in Applied Mechanics 29, 63–192. Keskar, N.R., Chelikowsky, J.R., 1992. Structural properties of nine silica polymorphs. Physical Review B 46, 1–13. Kimizuka, H., Kaburaki, H., Kogure, Y., 2000. Mechanism for negative Poisson ratios over the ˛-ˇ transition of cristobalite, SiO2 : A molecular-dynamics study. Physical Review Letters 84, 5548–5551. Lakes, R.S., Drugan, W.J., 2002. Dramatically stiffer elastic composite materials due to a negative stiffness phase? Journal of the Mechanics and Physics of Solids 50, 979–1009. Lakes, R.S., 1987. Foam structures with a negative Poisson’s ratio. Science 235, 1038–1040. Love, A.E.H., 1944. A Treatise on the Mathematical Theory of Elasticity, 4th edition. Dover Publications, New York, New York. Martin, P.A., 2003. On Green’s function for a bimaterial elastic half-plane. International Journal of Solids and Structures 40, 2101–2119. Smith, C.W., Grima, J.N., Evans, K.E., 2000. A novel mechanism for generating auxetic behaviour in reticulated foams: missing rib foam model. Acta Materialia 48, 4349–4356. Stavroulakis, G.E., 2005. Auxetic behavior: appearance and engineering applications. Physical Status Solidi B 242, 710–720. Tewary, V.K., 1991. Elastic Green’s function for a bi-material composite solid containing a free surface normal to the interface. Journal of Materials Research 6, 2592–2608. Ting, T.C.T., Chen, T., 2005. Poisson’s ratio for anisotropic elastic materials can have no bounds. Quarterly Journal of Mechanics and Applied Mathematics 58, 73–82. Williams, M.L., 1952. The stress around a fault or crack in dissimilar media. Bulletin of the Seismological Society of America 49, 199–204. Yang, W., Li, Z.-M., Shi, W., Xie, B.-H., Yang, M.-B., 2004. Review on auxetic materials. Journal of Materials Science 39, 3269–3279. Yeganeh-Haeri, A., Weidner, D.J., Parise, J.B., 1992. Elasticity of ˛-cristobalite: A silicon dioxide with a negative Poisson’s ratio. Science 257, 650–652.